#------------------------------------------------------------------------------
#$Date: 2026-05-02 00:37:25 +0200 (Sat, 02 May 2026) $
#$Revision: 305685 $
#$URL: svn://saulius.grazulis.lt/cod-secondary/cif/7/25/19/7251938.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7251938
loop_
_publ_author_name
'Kornyakov, Ilya V.'
'Bubnova, Olga'
'Kalinichev, Alexey A.'
'Likholetova, Marina V.'
'Krivovichev, Sergey V.'
_publ_section_title
;
 Subtle symmetry breaking in averievite-related compounds, (MX)Cu5O2(VO4)2
 (MX = CsBr, CsI, RbBr, RbI and KI)
;
_journal_name_full               CrystEngComm
_journal_paper_doi               10.1039/D5CE00495K
_journal_year                    2026
_chemical_formula_moiety         'Br Cs1 Cu5 O10 V2'
_chemical_formula_sum            'Br Cs Cu5 O10 V2'
_chemical_formula_weight         792.40
_space_group_crystal_system      trigonal
_space_group_IT_number           164
_space_group_name_Hall           '-P 3 2"'
_space_group_name_H-M_alt        'P -3 m 1'
_atom_sites_solution_primary     dual
_audit_creation_date             2025-02-17
_audit_creation_method
;
Olex2 1.5
(compiled 2024.02.16 svn.r378c4104 for OlexSys, GUI svn.r6928)
;
_audit_update_record
;
2025-05-13 deposited with the CCDC.	2026-04-30 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   6.38580(10)
_cell_length_b                   6.38580(10)
_cell_length_c                   8.3842(2)
_cell_measurement_reflns_used    11453
_cell_measurement_temperature    140(2)
_cell_measurement_theta_max      41.7600
_cell_measurement_theta_min      2.4600
_cell_volume                     296.089(10)
_computing_cell_refinement       'CrysAlisPro 1.171.42.102a (Rigaku OD, 2023)'
_computing_data_collection       'CrysAlisPro 1.171.42.102a (Rigaku OD, 2023)'
_computing_data_reduction        'CrysAlisPro 1.171.42.102a (Rigaku OD, 2023)'
_computing_molecular_graphics    'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.5 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2014/6 (Sheldrick, 2015)'
_diffrn_ambient_environment      N~2~
_diffrn_ambient_temperature      140(2)
_diffrn_detector                 'Hybrid Pixel Array Detector'
_diffrn_detector_area_resol_mean 10.0000
_diffrn_detector_type            HyPix
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 0.991
_diffrn_measurement_details
;
List of Runs (angles in degrees, time in seconds):

  # Type    Start    End  Width  tₑₓₚ   ω     θ     κ     φ   Frames
#--------------------------------------------------------------------------
  1  ω     17.00  85.00   0.50    1.00    --   34.02-133.00  -1.00  136
  2  ω    -63.00  39.00   0.50    1.00    --  -34.18  91.00 179.00  204
  3  ω    -23.00  67.00   0.50    1.00    --   34.02 -99.00-180.00  180
  4  ω     11.00  36.00   0.50    1.00    --   34.02  77.00 120.00   50
  5  ω     11.00 107.00   0.50    1.00    --   34.02  77.00-120.00  192
  6  ω    -17.00   8.00   0.50    1.00    --  -34.18   8.00-142.00   50
  7  ω     44.00  70.00   0.50    1.00    --   34.02 178.00 150.00   52
  8  ω     26.00  65.00   0.50    1.00    --   34.02  38.00  30.00   78
  9  ω     33.00 102.00   0.50    1.00    --   34.02  77.00 -90.00  138
 10  ω     42.00 107.00   0.50    1.00    --   34.02 178.00 120.00  130
 11  ω     13.00  67.00   0.50    1.00    --   34.02  73.00   6.00  108
 12  ω   -106.00 -19.00   0.50    1.00    --  -34.18 -57.00 120.00  174
 13  ω    -82.00 -56.00   0.50    1.00    --  -34.18 137.00-116.00   52
 14  ω     72.00 102.00   0.50    1.00    --   34.02  57.00 120.00   60
 15  ω      3.00  28.00   0.50    1.00    --   34.02  96.00-159.11   50
 16  ω     14.00  40.00   0.50    1.00    --   34.02  77.00  60.00   52
 17  ω     71.00 106.00   0.50    1.00    --   34.02  77.00  60.00   70
 18  ω      3.00  28.00   0.50    1.00    --   34.02  95.00 112.17   50
 19  ω    -28.00  -2.00   0.50    1.00    --   34.02 -19.00   0.00   52
 20  ω     22.00  61.00   0.50    1.00    --   34.02  57.00 120.00   78
 21  ω     20.00  89.00   0.50    1.00    --   34.02-137.00-178.00  138
 22  ω    -27.00  41.00   0.50    1.00    --  -34.18  19.00 -90.00  136
;
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type
'XtaLAB Synergy, Single source at home/near, HyPix'
_diffrn_measurement_method       'ω scans'
_diffrn_orient_matrix_type
'CrysAlisPro convention (1999,Acta A55,543-557)'
_diffrn_orient_matrix_UB_11      -0.0546926000
_diffrn_orient_matrix_UB_12      -0.0640351000
_diffrn_orient_matrix_UB_13      -0.0712351000
_diffrn_orient_matrix_UB_21      0.0879537000
_diffrn_orient_matrix_UB_22      0.0983404000
_diffrn_orient_matrix_UB_23      -0.0455885000
_diffrn_orient_matrix_UB_31      0.0756858000
_diffrn_orient_matrix_UB_32      -0.0517990000
_diffrn_orient_matrix_UB_33      0.0014718000
_diffrn_radiation_monochromator  mirror
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0603
_diffrn_reflns_av_unetI/netI     0.0182
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 0.991
_diffrn_reflns_limit_h_max       11
_diffrn_reflns_limit_h_min       -11
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            16341
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 0.991
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         41.780
_diffrn_reflns_theta_min         2.429
_diffrn_source                   'micro-focus sealed X-ray tube'
_diffrn_source_type              'PhotonJet (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    16.753
_exptl_absorpt_correction_T_max  0.398
_exptl_absorpt_correction_T_min  0.060
_exptl_absorpt_correction_type   gaussian
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.42.102a (Rigaku Oxford Diffraction, 2023)
Numerical absorption correction based on gaussian integration over
a multifaceted crystal model
Empirical absorption correction using spherical harmonics,
implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            black
_exptl_crystal_colour_primary    black
_exptl_crystal_density_diffrn    4.444
_exptl_crystal_description       plate
_exptl_crystal_F_000             361
_exptl_crystal_size_max          0.255
_exptl_crystal_size_mid          0.146
_exptl_crystal_size_min          0.103
_refine_diff_density_max         2.164
_refine_diff_density_min         -2.275
_refine_diff_density_rms         0.227
_refine_ls_extinction_coef       0.026(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.111
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     32
_refine_ls_number_reflns         810
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.111
_refine_ls_R_factor_all          0.0268
_refine_ls_R_factor_gt           0.0250
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0310P)²+0.5838P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0645
_refine_ls_wR_factor_ref         0.0652
_reflns_Friedel_coverage         0.000
_reflns_number_gt                761
_reflns_number_total             810
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            d5ce00495k2.cif
_cod_data_source_block           vcsbr_140_00
_cod_original_cell_volume        296.089(12)
_cod_database_code               7251938
_shelxl_version_number           2014/6
_chemical_oxdiff_formula         'Cs1 Br1 Cu5 V2 O10'
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_olex2_refinement_description
;
1. Others
 Sof(Cs1A)=0.08333*(1-FVAR(2))
 Sof(Cs1B)=0.08333*FVAR(2)
;
_olex2_submission_special_instructions 'No special instructions were received'
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
- Detector area scaling
- B-factor correction
;
_oxdiff_exptl_absorpt_empirical_full_max 3.117
_oxdiff_exptl_absorpt_empirical_full_min 0.635
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'y, x, -z'
'x-y, -y, -z'
'-x, -x+y, -z'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-y, -x, z'
'-x+y, y, z'
'x, x-y, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Cs1A Cs 1.0000 1.0000 1.0000 0.057(5) Uani 0.54(5) 12 d S T P . .
Cs1B Cs 1.0000 1.0000 0.9394(8) 0.0227(16) Uani 0.23(3) 6 d S T P . .
Br1 Br 1.0000 1.0000 0.5000 0.01634(11) Uani 1 12 d S T P . .
Cu1 Cu 0.3333 0.6667 0.22880(5) 0.00916(9) Uani 1 6 d S T P . .
Cu2 Cu 0.0000 0.5000 0.5000 0.00918(9) Uani 1 4 d S T P . .
V1 V 0.3333 0.6667 0.80608(6) 0.00456(9) Uani 1 6 d S T P . .
O1 O 0.3333 0.6667 1.0050(3) 0.0111(4) Uani 1 6 d S T P . .
O2 O 0.0374(3) 0.51868(14) 0.73725(18) 0.0131(3) Uani 1 2 d S T P . .
O3 O 0.3333 0.6667 0.4562(3) 0.0051(3) Uani 1 6 d S T P . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Br Br -0.2901 2.4595 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu 0.3201 1.2651 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
V V 0.3005 0.5294 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
1 -1 0 0.0766
9 -6 0 0.1096
0 8 0 0.0876
2 -9 0 0.0718
-7 -2 0 0.1062
-8 8 0 0.0688
0 0 -12 0.0513
0 0 12 0.0513
7 -6 6 0.0867
1 6 6 0.0835
3 -6 8 0.0675
-2 -4 10 0.0819
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
Cs1B Cs1A Cs1B 180.0 . 7_777 ?
Cs1B Cs1A V1 66.203(6) . 1_655 ?
Cs1B Cs1A V1 66.203(10) . . ?
Cs1B Cs1A V1 113.797(10) . 7_777 ?
Cs1B Cs1A V1 113.797(6) 7_777 1_655 ?
Cs1B Cs1A V1 113.797(6) . 7_677 ?
Cs1B Cs1A V1 113.797(10) 7_777 . ?
Cs1B Cs1A V1 66.203(6) 7_777 7_677 ?
Cs1B Cs1A V1 66.203(10) 7_777 7_777 ?
Cs1B Cs1A O1 89.35(4) . 7_677 ?
Cs1B Cs1A O1 89.35(4) . 7_667 ?
Cs1B Cs1A O1 90.65(4) . . ?
Cs1B Cs1A O1 89.35(4) 7_777 1_665 ?
Cs1B Cs1A O1 89.35(4) 7_777 1_655 ?
Cs1B Cs1A O1 90.65(4) 7_777 7_777 ?
Cs1B Cs1A O1 89.35(4) 7_777 . ?
Cs1B Cs1A O1 90.65(4) 7_777 7_677 ?
Cs1B Cs1A O1 90.65(4) 7_777 7_667 ?
Cs1B Cs1A O1 90.65(4) . 1_655 ?
Cs1B Cs1A O1 90.65(4) . 1_665 ?
Cs1B Cs1A O1 89.35(4) . 7_777 ?
V1 Cs1A V1 180.0 7_677 1_655 ?
V1 Cs1A V1 104.820(7) 1_655 . ?
V1 Cs1A V1 75.180(7) 7_677 . ?
V1 Cs1A V1 104.820(7) 7_677 7_777 ?
V1 Cs1A V1 180.0 . 7_777 ?
V1 Cs1A V1 75.180(7) 1_655 7_777 ?
O1 Cs1A V1 155.56(4) 7_677 1_655 ?
O1 Cs1A V1 155.56(4) . 7_777 ?
O1 Cs1A V1 117.517(16) 7_667 7_677 ?
O1 Cs1A V1 24.44(4) 1_655 1_655 ?
O1 Cs1A V1 117.517(16) 7_777 7_677 ?
O1 Cs1A V1 117.517(16) . 1_655 ?
O1 Cs1A V1 117.517(16) 7_677 7_777 ?
O1 Cs1A V1 62.483(16) 7_667 1_655 ?
O1 Cs1A V1 62.484(16) 1_665 7_777 ?
O1 Cs1A V1 117.517(16) 1_665 1_655 ?
O1 Cs1A V1 155.56(4) 7_777 . ?
O1 Cs1A V1 62.483(16) 7_777 1_655 ?
O1 Cs1A V1 62.483(16) 1_665 7_677 ?
O1 Cs1A V1 24.44(4) 7_677 7_677 ?
O1 Cs1A V1 62.483(16) 1_655 7_777 ?
O1 Cs1A V1 155.56(4) 1_655 7_677 ?
O1 Cs1A V1 117.516(16) 7_667 7_777 ?
O1 Cs1A V1 62.483(16) . 7_677 ?
O1 Cs1A V1 24.44(4) 7_777 7_777 ?
O1 Cs1A V1 62.483(16) 7_667 . ?
O1 Cs1A V1 117.517(16) 1_665 . ?
O1 Cs1A V1 62.483(16) 7_677 . ?
O1 Cs1A V1 117.517(16) 1_655 . ?
O1 Cs1A V1 24.44(4) . . ?
O1 Cs1A O1 60.012(2) 1_655 7_667 ?
O1 Cs1A O1 180.00(7) 7_677 1_655 ?
O1 Cs1A O1 119.987(2) 1_655 . ?
O1 Cs1A O1 60.013(2) 7_677 . ?
O1 Cs1A O1 60.013(2) . 7_667 ?
O1 Cs1A O1 119.988(2) 7_677 7_777 ?
O1 Cs1A O1 119.987(2) 7_667 7_777 ?
O1 Cs1A O1 119.988(2) 1_655 1_665 ?
O1 Cs1A O1 60.013(2) 1_665 7_777 ?
O1 Cs1A O1 119.987(2) . 1_665 ?
O1 Cs1A O1 119.988(2) 7_677 7_667 ?
O1 Cs1A O1 60.012(2) 1_655 7_777 ?
O1 Cs1A O1 180.00(7) 7_667 1_665 ?
O1 Cs1A O1 180.0 . 7_777 ?
O1 Cs1A O1 60.012(2) 7_677 1_665 ?
Cs1A Cs1B Cs1B 0.000(4) . 7_777 ?
Cs1A Cs1B Br1 180.0 . . ?
Cs1A Cs1B O1 82.79(11) . 7_677 ?
Cs1A Cs1B O1 82.79(11) . 7_777 ?
Cs1A Cs1B O1 82.79(11) . 7_667 ?
Cs1A Cs1B O2 117.92(10) . 3_665 ?
Cs1A Cs1B O2 117.92(10) . 1_655 ?
Cs1A Cs1B O2 117.92(10) . 2_775 ?
Cs1A Cs1B O2 117.92(10) . 3_565 ?
Cs1A Cs1B O2 117.92(10) . 2_665 ?
Cs1A Cs1B O2 117.92(10) . 1_665 ?
Cs1B Cs1B Br1 180.0 7_777 . ?
Cs1B Cs1B O1 82.79(12) 7_777 7_777 ?
Cs1B Cs1B O1 82.79(11) 7_777 7_667 ?
Cs1B Cs1B O1 82.79(11) 7_777 7_677 ?
Cs1B Cs1B O2 117.92(10) 7_777 3_565 ?
Cs1B Cs1B O2 117.92(10) 7_777 2_775 ?
Cs1B Cs1B O2 117.92(10) 7_777 1_655 ?
Cs1B Cs1B O2 117.92(10) 7_777 1_665 ?
Cs1B Cs1B O2 117.92(10) 7_777 3_665 ?
Cs1B Cs1B O2 117.92(10) 7_777 2_665 ?
Br1 Cs1B O1 97.21(11) . 7_677 ?
Br1 Cs1B O1 97.21(11) . 7_667 ?
Br1 Cs1B O1 97.21(11) . 7_777 ?
O1 Cs1B O1 118.45(5) 7_777 7_667 ?
O1 Cs1B O1 118.45(5) 7_677 7_667 ?
O1 Cs1B O1 118.45(5) 7_677 7_777 ?
O2 Cs1B Br1 62.08(10) 1_665 . ?
O2 Cs1B Br1 62.08(10) 3_665 . ?
O2 Cs1B Br1 62.08(10) 3_565 . ?
O2 Cs1B Br1 62.08(10) 2_775 . ?
O2 Cs1B Br1 62.08(10) 1_655 . ?
O2 Cs1B Br1 62.08(10) 2_665 . ?
O2 Cs1B O1 47.89(4) 3_565 7_677 ?
O2 Cs1B O1 90.12(5) 3_665 7_667 ?
O2 Cs1B O1 147.64(14) 1_665 7_667 ?
O2 Cs1B O1 47.89(4) 1_665 7_677 ?
O2 Cs1B O1 47.89(4) 3_665 7_777 ?
O2 Cs1B O1 90.12(5) 2_665 7_677 ?
O2 Cs1B O1 147.63(13) 2_775 7_667 ?
O2 Cs1B O1 90.12(5) 2_775 7_677 ?
O2 Cs1B O1 90.12(5) 1_655 7_777 ?
O2 Cs1B O1 147.64(14) 1_655 7_677 ?
O2 Cs1B O1 90.12(5) 3_565 7_667 ?
O2 Cs1B O1 147.64(13) 3_665 7_677 ?
O2 Cs1B O1 47.89(4) 2_665 7_667 ?
O2 Cs1B O1 147.64(14) 3_565 7_777 ?
O2 Cs1B O1 47.89(4) 1_655 7_667 ?
O2 Cs1B O1 90.12(5) 1_665 7_777 ?
O2 Cs1B O1 47.89(4) 2_775 7_777 ?
O2 Cs1B O1 147.63(13) 2_665 7_777 ?
O2 Cs1B O2 123.7(2) 3_565 3_665 ?
O2 Cs1B O2 99.86(13) 3_565 2_775 ?
O2 Cs1B O2 99.86(13) 3_565 1_655 ?
O2 Cs1B O2 46.09(7) 1_655 3_665 ?
O2 Cs1B O2 58.72(8) 2_665 1_655 ?
O2 Cs1B O2 46.09(7) 1_665 2_775 ?
O2 Cs1B O2 46.09(7) 3_565 2_665 ?
O2 Cs1B O2 123.7(2) 2_665 2_775 ?
O2 Cs1B O2 123.7(2) 1_665 1_655 ?
O2 Cs1B O2 99.86(13) 1_665 2_665 ?
O2 Cs1B O2 58.72(8) 3_565 1_665 ?
O2 Cs1B O2 99.86(13) 2_665 3_665 ?
O2 Cs1B O2 99.86(13) 2_775 1_655 ?
O2 Cs1B O2 58.72(8) 2_775 3_665 ?
O2 Cs1B O2 99.86(13) 1_665 3_665 ?
Cs1A Br1 Cs1A 180.0 . 1_554 ?
Cs1B Br1 Cs1A 180.0 . 1_554 ?
Cs1B Br1 Cs1A 180.0 7_776 . ?
Cs1B Br1 Cs1A 0.000(1) . . ?
Cs1B Br1 Cs1A 0.0 7_776 1_554 ?
Cs1B Br1 Cs1B 180.0 7_776 . ?
Cs1B Cu1 Cs1A 104.44(6) 7_666 1_454 ?
Cs1B Cu1 Cs1A 6.55(10) 7_676 1_454 ?
Cs1B Cu1 Cs1A 104.44(6) 7_776 1_454 ?
Cs1B Cu1 Cs1B 107.97(10) 7_676 7_666 ?
Cs1B Cu1 Cs1B 107.97(10) 7_666 7_776 ?
Cs1B Cu1 Cs1B 107.97(10) 7_676 7_776 ?
Cu2 Cu1 Cs1A 94.543(1) . 1_454 ?
Cu2 Cu1 Cs1A 94.543(2) 3_565 1_454 ?
Cu2 Cu1 Cs1A 156.521(9) 2_665 1_454 ?
Cu2 Cu1 Cs1B 149.97(10) . 7_776 ?
Cu2 Cu1 Cs1B 89.05(8) 3_565 7_676 ?
Cu2 Cu1 Cs1B 89.05(8) 2_665 7_666 ?
Cu2 Cu1 Cs1B 89.05(8) 2_665 7_776 ?
Cu2 Cu1 Cs1B 89.05(8) . 7_676 ?
Cu2 Cu1 Cs1B 149.97(10) 2_665 7_676 ?
Cu2 Cu1 Cs1B 149.97(10) 3_565 7_666 ?
Cu2 Cu1 Cs1B 89.05(8) . 7_666 ?
Cu2 Cu1 Cs1B 89.05(8) 3_565 7_776 ?
Cu2 Cu1 Cu2 66.102(8) 3_565 . ?
Cu2 Cu1 Cu2 66.102(8) 3_565 2_665 ?
Cu2 Cu1 Cu2 66.102(8) . 2_665 ?
O1 Cu1 Cs1A 62.511(5) 1_554 1_454 ?
O1 Cu1 Cs1B 69.06(10) 1_554 7_776 ?
O1 Cu1 Cs1B 69.06(10) 1_554 7_666 ?
O1 Cu1 Cs1B 69.06(10) 1_554 7_676 ?
O1 Cu1 Cu2 140.967(5) 1_554 3_565 ?
O1 Cu1 Cu2 140.967(5) 1_554 . ?
O1 Cu1 Cu2 140.968(5) 1_554 2_665 ?
O1 Cu1 O2 97.91(4) 1_554 7_566 ?
O1 Cu1 O2 97.91(4) 1_554 8_556 ?
O1 Cu1 O2 97.91(4) 1_554 9_666 ?
O1 Cu1 O3 180.0 1_554 . ?
O2 Cu1 Cs1A 67.92(2) 7_566 1_454 ?
O2 Cu1 Cs1A 160.42(4) 8_556 1_454 ?
O2 Cu1 Cs1A 67.92(2) 9_666 1_454 ?
O2 Cu1 Cs1B 65.58(4) 8_556 7_666 ?
O2 Cu1 Cs1B 65.58(4) 8_556 7_776 ?
O2 Cu1 Cs1B 65.58(4) 9_666 7_776 ?
O2 Cu1 Cs1B 65.58(4) 7_566 7_676 ?
O2 Cu1 Cs1B 166.97(11) 8_556 7_676 ?
O2 Cu1 Cs1B 166.97(11) 7_566 7_776 ?
O2 Cu1 Cs1B 65.58(4) 9_666 7_676 ?
O2 Cu1 Cs1B 166.97(11) 9_666 7_666 ?
O2 Cu1 Cs1B 65.58(4) 7_566 7_666 ?
O2 Cu1 Cu2 101.83(4) 9_666 2_665 ?
O2 Cu1 Cu2 101.83(4) 7_566 3_565 ?
O2 Cu1 Cu2 43.06(4) 7_566 . ?
O2 Cu1 Cu2 101.83(4) 7_566 2_665 ?
O2 Cu1 Cu2 101.83(4) 8_556 3_565 ?
O2 Cu1 Cu2 43.06(4) 8_556 2_665 ?
O2 Cu1 Cu2 101.83(4) 8_556 . ?
O2 Cu1 Cu2 43.06(4) 9_666 3_565 ?
O2 Cu1 Cu2 101.83(4) 9_666 . ?
O2 Cu1 O2 118.14(2) 9_666 8_556 ?
O2 Cu1 O2 118.14(2) 7_566 8_556 ?
O2 Cu1 O2 118.14(2) 9_666 7_566 ?
O3 Cu1 Cs1A 117.488(5) . 1_454 ?
O3 Cu1 Cs1B 110.94(10) . 7_666 ?
O3 Cu1 Cs1B 110.94(10) . 7_676 ?
O3 Cu1 Cs1B 110.94(10) . 7_776 ?
O3 Cu1 Cu2 39.032(5) . 3_565 ?
O3 Cu1 Cu2 39.032(5) . 2_665 ?
O3 Cu1 Cu2 39.032(5) . . ?
O3 Cu1 O2 82.09(4) . 7_566 ?
O3 Cu1 O2 82.09(4) . 8_556 ?
O3 Cu1 O2 82.09(4) . 9_666 ?
Cu1 Cu2 Cu1 180.0 . 7_566 ?
O2 Cu2 Cu1 135.04(4) 7_566 7_566 ?
O2 Cu2 Cu1 135.04(4) . . ?
O2 Cu2 Cu1 44.96(4) . 7_566 ?
O2 Cu2 Cu1 44.96(4) 7_566 . ?
O2 Cu2 O2 180.0 . 7_566 ?
O3 Cu2 Cu1 140.30(6) 7_566 . ?
O3 Cu2 Cu1 39.70(6) . . ?
O3 Cu2 Cu1 140.30(6) . 7_566 ?
O3 Cu2 Cu1 39.70(6) 7_566 7_566 ?
O3 Cu2 O2 84.66(8) 7_566 . ?
O3 Cu2 O2 84.66(8) . 7_566 ?
O3 Cu2 O2 95.34(8) . . ?
O3 Cu2 O2 95.34(8) 7_566 7_566 ?
O3 Cu2 O3 180.0 7_566 . ?
Cs1A V1 Cs1A 104.820(7) 1_455 1_445 ?
Cs1A V1 Cs1A 104.820(7) . 1_445 ?
Cs1A V1 Cs1A 104.820(7) 1_455 . ?
Cs1A V1 Cs1B 101.18(5) 1_445 7_777 ?
Cs1A V1 Cs1B 6.26(8) 1_455 7_677 ?
Cs1A V1 Cs1B 101.18(5) . 7_677 ?
Cs1A V1 Cs1B 101.18(5) 1_445 7_677 ?
Cs1A V1 Cs1B 101.18(5) 1_455 7_777 ?
Cs1A V1 Cs1B 6.26(8) . 7_777 ?
Cs1B V1 Cs1A 6.93(10) . . ?
Cs1B V1 Cs1A 108.71(6) . 1_445 ?
Cs1B V1 Cs1A 108.71(6) 1_445 . ?
Cs1B V1 Cs1A 108.71(6) . 1_455 ?
Cs1B V1 Cs1A 108.71(6) 1_455 1_445 ?
Cs1B V1 Cs1A 6.93(10) 1_455 1_455 ?
Cs1B V1 Cs1A 108.71(6) 1_455 . ?
Cs1B V1 Cs1A 108.71(6) 1_445 1_455 ?
Cs1B V1 Cs1A 6.93(10) 1_445 1_445 ?
Cs1B V1 Cs1B 111.94(9) 1_455 1_445 ?
Cs1B V1 Cs1B 111.94(9) 1_445 . ?
Cs1B V1 Cs1B 105.59(2) 1_445 7_677 ?
Cs1B V1 Cs1B 111.94(9) 1_455 . ?
Cs1B V1 Cs1B 97.10(11) 7_677 7_777 ?
Cs1B V1 Cs1B 105.59(2) 1_455 7_777 ?
Cs1B V1 Cs1B 105.59(2) . 7_677 ?
Cs1B V1 Cs1B 105.59(2) 1_445 7_777 ?
Cs1B V1 Cs1B 13.19(18) . 7_777 ?
Cs1B V1 Cs1B 13.19(18) 1_455 7_677 ?
O1 V1 Cs1A 66.203(6) . . ?
O1 V1 Cs1A 66.203(6) . 1_455 ?
O1 V1 Cs1A 66.203(6) . 1_445 ?
O1 V1 Cs1B 73.13(10) . 1_455 ?
O1 V1 Cs1B 59.94(8) . 7_777 ?
O1 V1 Cs1B 73.13(10) . . ?
O1 V1 Cs1B 73.13(10) . 1_445 ?
O1 V1 Cs1B 59.94(8) . 7_677 ?
O1 V1 O2 109.42(5) . 3_565 ?
O1 V1 O2 109.42(5) . . ?
O1 V1 O2 109.42(5) . 2_665 ?
O2 V1 Cs1A 72.71(3) 2_665 . ?
O2 V1 Cs1A 175.63(5) . . ?
O2 V1 Cs1A 72.71(3) . 1_445 ?
O2 V1 Cs1A 175.62(5) 2_665 1_455 ?
O2 V1 Cs1A 175.63(5) 3_565 1_445 ?
O2 V1 Cs1A 72.71(3) 3_565 1_455 ?
O2 V1 Cs1A 72.71(3) 2_665 1_445 ?
O2 V1 Cs1A 72.71(3) . 1_455 ?
O2 V1 Cs1A 72.70(3) 3_565 . ?
O2 V1 Cs1B 69.22(6) 2_665 1_445 ?
O2 V1 Cs1B 76.02(5) 3_565 7_677 ?
O2 V1 Cs1B 169.36(10) . 7_777 ?
O2 V1 Cs1B 177.45(11) . . ?
O2 V1 Cs1B 76.02(6) . 7_677 ?
O2 V1 Cs1B 69.22(6) 2_665 . ?
O2 V1 Cs1B 76.02(6) 2_665 7_777 ?
O2 V1 Cs1B 177.45(11) 3_565 1_445 ?
O2 V1 Cs1B 69.22(5) . 1_455 ?
O2 V1 Cs1B 69.22(5) 3_565 1_455 ?
O2 V1 Cs1B 177.45(11) 2_665 1_455 ?
O2 V1 Cs1B 76.02(6) 3_565 7_777 ?
O2 V1 Cs1B 69.22(6) . 1_445 ?
O2 V1 Cs1B 69.22(6) 3_565 . ?
O2 V1 Cs1B 169.36(10) 2_665 7_677 ?
O2 V1 O2 109.52(5) 3_565 . ?
O2 V1 O2 109.52(5) 3_565 2_665 ?
O2 V1 O2 109.52(5) . 2_665 ?
Cs1A O1 Cs1A 119.987(1) 1_455 . ?
Cs1A O1 Cs1A 119.987(1) 1_455 1_445 ?
Cs1A O1 Cs1A 119.987(2) 1_445 . ?
Cs1A O1 Cs1B 119.528(15) 1_445 1_455 ?
Cs1A O1 Cs1B 119.528(15) 1_455 . ?
Cs1A O1 Cs1B 119.528(15) 1_455 1_445 ?
Cs1A O1 Cs1B 119.830(10) . 7_667 ?
Cs1A O1 Cs1B 119.528(15) . 1_445 ?
Cs1A O1 Cs1B 7.85(11) 1_455 7_677 ?
Cs1A O1 Cs1B 7.85(11) 1_445 7_667 ?
Cs1A O1 Cs1B 119.830(11) 1_445 7_677 ?
Cs1A O1 Cs1B 7.83(11) 1_455 1_455 ?
Cs1A O1 Cs1B 119.830(11) . 7_677 ?
Cs1A O1 Cs1B 119.528(15) . 1_455 ?
Cs1A O1 Cs1B 119.830(11) 1_455 7_667 ?
Cs1A O1 Cs1B 119.528(14) 1_445 . ?
Cs1A O1 Cs1B 119.830(11) 1_455 7_777 ?
Cs1A O1 Cs1B 7.83(11) 1_445 1_445 ?
Cs1A O1 Cs1B 119.830(10) 1_445 7_777 ?
Cs1A O1 Cs1B 7.85(11) . 7_777 ?
Cs1A O1 Cs1B 7.83(11) . . ?
Cs1B O1 Cs1B 118.45(5) 7_677 7_777 ?
Cs1B O1 Cs1B 117.87(6) 1_455 . ?
Cs1B O1 Cs1B 120.605(17) 7_777 1_445 ?
Cs1B O1 Cs1B 15.7(2) 7_677 1_455 ?
Cs1B O1 Cs1B 118.45(5) 7_777 7_667 ?
Cs1B O1 Cs1B 120.605(18) 7_777 1_455 ?
Cs1B O1 Cs1B 120.605(18) 7_667 . ?
Cs1B O1 Cs1B 120.605(19) 7_667 1_455 ?
Cs1B O1 Cs1B 118.45(5) 7_677 7_667 ?
Cs1B O1 Cs1B 117.87(6) 1_455 1_445 ?
Cs1B O1 Cs1B 120.61(2) 7_677 1_445 ?
Cs1B O1 Cs1B 117.87(6) . 1_445 ?
Cs1B O1 Cs1B 15.7(2) 7_667 1_445 ?
Cs1B O1 Cs1B 15.7(2) 7_777 . ?
Cs1B O1 Cs1B 120.605(19) 7_677 . ?
Cu1 O1 Cs1A 90.65(4) 1_556 1_445 ?
Cu1 O1 Cs1A 90.65(4) 1_556 . ?
Cu1 O1 Cs1A 90.65(4) 1_556 1_455 ?
Cu1 O1 Cs1B 98.47(12) 1_556 1_445 ?
Cu1 O1 Cs1B 82.79(11) 1_556 7_677 ?
Cu1 O1 Cs1B 82.79(12) 1_556 7_667 ?
Cu1 O1 Cs1B 98.47(12) 1_556 . ?
Cu1 O1 Cs1B 98.47(11) 1_556 1_455 ?
Cu1 O1 Cs1B 82.79(12) 1_556 7_777 ?
V1 O1 Cs1A 89.35(4) . 1_455 ?
V1 O1 Cs1A 89.35(4) . 1_445 ?
V1 O1 Cs1A 89.35(4) . . ?
V1 O1 Cs1B 97.21(11) . 7_677 ?
V1 O1 Cs1B 81.53(12) . . ?
V1 O1 Cs1B 81.53(12) . 1_445 ?
V1 O1 Cs1B 81.53(11) . 1_455 ?
V1 O1 Cs1B 97.21(12) . 7_667 ?
V1 O1 Cs1B 97.21(12) . 7_777 ?
V1 O1 Cu1 180.0 . 1_556 ?
Cs1B O2 Cs1B 123.7(2) 1_455 1_445 ?
Cu1 O2 Cs1B 83.05(3) 7_566 1_445 ?
Cu1 O2 Cs1B 83.06(3) 7_566 1_455 ?
Cu2 O2 Cs1B 117.37(10) . 1_455 ?
Cu2 O2 Cs1B 117.37(10) . 1_445 ?
Cu2 O2 Cu1 91.98(6) . 7_566 ?
V1 O2 Cs1B 84.15(5) . 1_445 ?
V1 O2 Cs1B 84.15(5) . 1_455 ?
V1 O2 Cu1 152.67(9) . 7_566 ?
V1 O2 Cu2 115.35(8) . . ?
Cu2 O3 Cu1 101.27(6) 3_565 . ?
Cu2 O3 Cu1 101.27(6) . . ?
Cu2 O3 Cu1 101.27(6) 2_665 . ?
Cu2 O3 Cu2 116.28(4) . 2_665 ?
Cu2 O3 Cu2 116.28(4) 3_565 2_665 ?
Cu2 O3 Cu2 116.28(4) 3_565 . ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Cs1A Cs1B 0.508(7) . ?
Cs1A Cs1B 0.508(7) 7_777 ?
Cs1A V1 4.0294(2) 7_777 ?
Cs1A V1 4.0294(2) 1_655 ?
Cs1A V1 4.0294(2) 7_677 ?
Cs1A V1 4.0294(2) . ?
Cs1A O1 3.68709(8) 1_665 ?
Cs1A O1 3.68708(7) . ?
Cs1A O1 3.68706(7) 1_655 ?
Cs1A O1 3.68709(7) 7_777 ?
Cs1A O1 3.68709(7) 7_667 ?
Cs1A O1 3.68706(6) 7_677 ?
Cs1B Cs1B 1.015(14) 7_777 ?
Cs1B Br1 3.684(7) . ?
Cs1B O1 3.7162(9) 7_667 ?
Cs1B O1 3.7162(9) 7_677 ?
Cs1B O1 3.7162(9) 7_777 ?
Cs1B O2 3.621(3) 3_665 ?
Cs1B O2 3.621(3) 1_665 ?
Cs1B O2 3.621(3) 2_775 ?
Cs1B O2 3.621(3) 1_655 ?
Cs1B O2 3.621(3) 3_565 ?
Cs1B O2 3.621(3) 2_665 ?
Br1 Cs1A 4.19210(11) 1_554 ?
Br1 Cs1B 3.684(7) 7_776 ?
Cu1 Cs1A 4.15604(18) 1_454 ?
Cu1 Cs1B 3.947(3) 7_666 ?
Cu1 Cs1B 3.947(3) 7_676 ?
Cu1 Cs1B 3.947(3) 7_776 ?
Cu1 Cu2 2.9272(3) 3_565 ?
Cu1 Cu2 2.9272(3) . ?
Cu1 Cu2 2.9272(3) 2_665 ?
Cu1 O1 1.877(2) 1_554 ?
Cu1 O2 2.0697(15) 8_556 ?
Cu1 O2 2.0697(15) 9_666 ?
Cu1 O2 2.0697(15) 7_566 ?
Cu1 O3 1.907(2) . ?
Cu2 Cu1 2.9272(3) 7_566 ?
Cu2 O2 1.9998(15) . ?
Cu2 O2 1.9998(15) 7_566 ?
Cu2 O3 1.8796(4) 7_566 ?
Cu2 O3 1.8796(4) . ?
V1 Cs1A 4.0294(2) 1_445 ?
V1 Cs1A 4.0294(2) 1_455 ?
V1 Cs1B 3.853(2) 1_455 ?
V1 Cs1B 4.260(4) 7_677 ?
V1 Cs1B 4.260(4) 7_777 ?
V1 Cs1B 3.853(2) 1_445 ?
V1 O1 1.667(2) . ?
V1 O2 1.7356(16) . ?
V1 O2 1.7355(16) 3_565 ?
V1 O2 1.7356(15) 2_665 ?
O1 Cs1A 3.68708(7) 1_455 ?
O1 Cs1A 3.68708(7) 1_445 ?
O1 Cs1B 3.7162(9) 7_677 ?
O1 Cs1B 3.7162(10) 7_667 ?
O1 Cs1B 3.7275(11) 1_455 ?
O1 Cs1B 3.7162(10) 7_777 ?
O1 Cs1B 3.7275(11) 1_445 ?
O1 Cu1 1.877(2) 1_556 ?
O2 Cs1B 3.621(3) 1_445 ?
O2 Cs1B 3.621(3) 1_455 ?
O2 Cu1 2.0697(15) 7_566 ?
O3 Cu2 1.8796(4) 2_665 ?
O3 Cu2 1.8797(4) 3_565 ?
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
Cs1A V1 O1 Cs1A 120.000(0) . . . 1_455 ?
Cs1A V1 O1 Cs1A -120.000(0) 1_455 . . . ?
Cs1A V1 O1 Cs1A -120.000(0) . . . 1_445 ?
Cs1A V1 O1 Cs1A -120.000(0) 1_445 . . 1_455 ?
Cs1A V1 O1 Cs1A 120.000(0) 1_455 . . 1_445 ?
Cs1A V1 O1 Cs1A 120.000(0) 1_445 . . . ?
Cs1A V1 O1 Cs1B -120.000(1) . . . 7_667 ?
Cs1A V1 O1 Cs1B 120.000(1) 1_455 . . 1_445 ?
Cs1A V1 O1 Cs1B 0.000(0) . . . . ?
Cs1A V1 O1 Cs1B 0.000(1) 1_455 . . 1_455 ?
Cs1A V1 O1 Cs1B 0.000(0) 1_445 . . 1_445 ?
Cs1A V1 O1 Cs1B -120.000(1) 1_445 . . 1_455 ?
Cs1A V1 O1 Cs1B 0.000(0) 1_445 . . 7_667 ?
Cs1A V1 O1 Cs1B 0.000(1) 1_455 . . 7_677 ?
Cs1A V1 O1 Cs1B 120.000(1) . . . 1_455 ?
Cs1A V1 O1 Cs1B 120.000(1) . . . 7_677 ?
Cs1A V1 O1 Cs1B -120.000(0) 1_455 . . . ?
Cs1A V1 O1 Cs1B -120.000(0) 1_455 . . 7_777 ?
Cs1A V1 O1 Cs1B 120.000(0) 1_445 . . . ?
Cs1A V1 O1 Cs1B 0.000(0) . . . 7_777 ?
Cs1A V1 O1 Cs1B -120.000(1) . . . 1_445 ?
Cs1A V1 O1 Cs1B 120.000(0) 1_445 . . 7_777 ?
Cs1A V1 O1 Cs1B 120.000(1) 1_455 . . 7_667 ?
Cs1A V1 O1 Cs1B -120.000(1) 1_445 . . 7_677 ?
Cs1A V1 O2 Cs1B 6.33(10) 1_455 . . 1_455 ?
Cs1A V1 O2 Cs1B -6.33(9) 1_445 . . 1_445 ?
Cs1A V1 O2 Cs1B -118.51(10) 1_455 . . 1_445 ?
Cs1A V1 O2 Cs1B 118.52(10) 1_445 . . 1_455 ?
Cs1A V1 O2 Cu1 -56.092(13) 1_455 . . 7_566 ?
Cs1A V1 O2 Cu1 56.089(13) 1_445 . . 7_566 ?
Cs1A V1 O2 Cu2 123.910(13) 1_455 . . . ?
Cs1A V1 O2 Cu2 -123.910(13) 1_445 . . . ?
Cs1B V1 O1 Cs1A 0.000(0) 7_677 . . 1_455 ?
Cs1B V1 O1 Cs1A 120.000(0) 1_455 . . 1_445 ?
Cs1B V1 O1 Cs1A -120.000(0) 1_455 . . . ?
Cs1B V1 O1 Cs1A 120.0 1_445 . . . ?
Cs1B V1 O1 Cs1A 0.000(0) 1_455 . . 1_455 ?
Cs1B V1 O1 Cs1A 0.0 . . . . ?
Cs1B V1 O1 Cs1A 120.000(0) 7_677 . . 1_445 ?
Cs1B V1 O1 Cs1A -120.0 . . . 1_445 ?
Cs1B V1 O1 Cs1A -120.0 1_445 . . 1_455 ?
Cs1B V1 O1 Cs1A 120.0 . . . 1_455 ?
Cs1B V1 O1 Cs1A 120.000(0) 7_777 . . 1_455 ?
Cs1B V1 O1 Cs1A -120.000(0) 7_677 . . . ?
Cs1B V1 O1 Cs1A 0.0 1_445 . . 1_445 ?
Cs1B V1 O1 Cs1A 0.000(0) 7_777 . . . ?
Cs1B V1 O1 Cs1A -120.000(0) 7_777 . . 1_445 ?
Cs1B V1 O1 Cs1B 0.000(1) 1_455 . . 7_677 ?
Cs1B V1 O1 Cs1B -120.000(0) 1_455 . . . ?
Cs1B V1 O1 Cs1B -120.000(1) 7_777 . . 7_667 ?
Cs1B V1 O1 Cs1B -120.000(1) 1_445 . . 7_677 ?
Cs1B V1 O1 Cs1B 120.000(0) 1_455 . . 1_445 ?
Cs1B V1 O1 Cs1B 120.000(1) . . . 7_677 ?
Cs1B V1 O1 Cs1B 0.000(1) 7_677 . . 1_455 ?
Cs1B V1 O1 Cs1B 120.000(1) 7_777 . . 7_677 ?
Cs1B V1 O1 Cs1B -120.000(0) 7_677 . . . ?
Cs1B V1 O1 Cs1B -120.000(0) 1_455 . . 7_777 ?
Cs1B V1 O1 Cs1B 120.000(1) 7_677 . . 1_445 ?
Cs1B V1 O1 Cs1B 120.000(0) 1_445 . . 7_777 ?
Cs1B V1 O1 Cs1B 120.000(1) . . . 1_455 ?
Cs1B V1 O1 Cs1B 0.000(0) . . . 7_777 ?
Cs1B V1 O1 Cs1B 120.000(1) 7_777 . . 1_455 ?
Cs1B V1 O1 Cs1B -120.000(1) 7_677 . . 7_777 ?
Cs1B V1 O1 Cs1B 120.000(0) 1_445 . . . ?
Cs1B V1 O1 Cs1B 120.000(1) 1_455 . . 7_667 ?
Cs1B V1 O1 Cs1B 0.000(0) 7_777 . . . ?
Cs1B V1 O1 Cs1B 0.000(0) 1_445 . . 7_667 ?
Cs1B V1 O1 Cs1B -120.000(1) . . . 1_445 ?
Cs1B V1 O1 Cs1B -120.000(1) . . . 7_667 ?
Cs1B V1 O1 Cs1B -120.000(1) 7_777 . . 1_445 ?
Cs1B V1 O1 Cs1B 120.000(1) 7_677 . . 7_667 ?
Cs1B V1 O1 Cs1B -120.000(1) 1_445 . . 1_455 ?
Cs1B V1 O2 Cs1B -62.42(10) 7_777 . . 1_445 ?
Cs1B V1 O2 Cs1B -124.85(19) 1_455 . . 1_445 ?
Cs1B V1 O2 Cs1B 62.42(10) 7_777 . . 1_455 ?
Cs1B V1 O2 Cs1B -113.00(3) 7_677 . . 1_445 ?
Cs1B V1 O2 Cs1B 11.85(17) 7_677 . . 1_455 ?
Cs1B V1 O2 Cs1B 124.85(19) 1_445 . . 1_455 ?
Cs1B V1 O2 Cu1 -62.43(10) 1_455 . . 7_566 ?
Cs1B V1 O2 Cu1 -50.57(7) 7_677 . . 7_566 ?
Cs1B V1 O2 Cu1 62.42(10) 1_445 . . 7_566 ?
Cs1B V1 O2 Cu1 -0.001(1) 7_777 . . 7_566 ?
Cs1B V1 O2 Cu2 129.43(7) 7_677 . . . ?
Cs1B V1 O2 Cu2 -117.58(10) 1_445 . . . ?
Cs1B V1 O2 Cu2 180.000(1) 7_777 . . . ?
Cs1B V1 O2 Cu2 117.58(10) 1_455 . . . ?
Cu1 Cu2 O3 Cu1 180.0 7_566 . . . ?
Cu1 Cu2 O3 Cu2 71.30(10) 7_566 . . 2_665 ?
Cu1 Cu2 O3 Cu2 108.70(10) . . . 3_565 ?
Cu1 Cu2 O3 Cu2 -71.30(10) 7_566 . . 3_565 ?
Cu1 Cu2 O3 Cu2 -108.70(10) . . . 2_665 ?
V1 Cs1A Cs1B Cs1B 150.0(2) 1_655 . . 7_777 ?
V1 Cs1A Cs1B Cs1B 150.00(1) 7_677 . . 7_777 ?
V1 Cs1A Cs1B Cs1B 30.0(2) . . . 7_777 ?
V1 Cs1A Cs1B Cs1B -150.0(2) 7_777 . . 7_777 ?
V1 Cs1A Cs1B O1 -60.000(3) 1_655 . . 7_777 ?
V1 Cs1A Cs1B O1 0.000(1) 7_777 . . 7_777 ?
V1 Cs1A Cs1B O1 120.000(4) 7_677 . . 7_777 ?
V1 Cs1A Cs1B O1 119.999(0) 7_777 . . 7_667 ?
V1 Cs1A Cs1B O1 -60.000(1) . . . 7_667 ?
V1 Cs1A Cs1B O1 0.000(2) 7_677 . . 7_677 ?
V1 Cs1A Cs1B O1 180.000(1) . . . 7_777 ?
V1 Cs1A Cs1B O1 180.000(2) 1_655 . . 7_677 ?
V1 Cs1A Cs1B O1 60.000(4) 1_655 . . 7_667 ?
V1 Cs1A Cs1B O1 60.000(2) . . . 7_677 ?
V1 Cs1A Cs1B O1 -120.000(2) 7_777 . . 7_677 ?
V1 Cs1A Cs1B O1 -120.000(4) 7_677 . . 7_667 ?
V1 Cs1A Cs1B O2 86.30(3) 7_777 . . 1_655 ?
V1 Cs1A Cs1B O2 -86.30(3) 7_677 . . 2_665 ?
V1 Cs1A Cs1B O2 146.30(3) . . . 2_775 ?
V1 Cs1A Cs1B O2 -33.70(3) 7_677 . . 3_565 ?
V1 Cs1A Cs1B O2 86.30(3) 7_677 . . 2_775 ?
V1 Cs1A Cs1B O2 146.30(3) 1_655 . . 3_565 ?
V1 Cs1A Cs1B O2 -86.30(3) 7_777 . . 1_665 ?
V1 Cs1A Cs1B O2 26.30(3) . . . 3_565 ?
V1 Cs1A Cs1B O2 -26.30(3) . . . 2_665 ?
V1 Cs1A Cs1B O2 -153.70(3) 7_777 . . 3_565 ?
V1 Cs1A Cs1B O2 26.30(3) 1_655 . . 1_655 ?
V1 Cs1A Cs1B O2 -26.30(3) 1_655 . . 3_665 ?
V1 Cs1A Cs1B O2 -33.70(3) 7_777 . . 2_775 ?
V1 Cs1A Cs1B O2 -146.30(3) . . . 3_665 ?
V1 Cs1A Cs1B O2 -93.70(3) . . . 1_655 ?
V1 Cs1A Cs1B O2 33.70(3) 7_777 . . 3_665 ?
V1 Cs1A Cs1B O2 93.70(3) 1_655 . . 2_665 ?
V1 Cs1A Cs1B O2 33.70(3) 7_677 . . 1_665 ?
V1 Cs1A Cs1B O2 153.70(3) 7_777 . . 2_665 ?
V1 Cs1A Cs1B O2 -146.30(3) 1_655 . . 1_665 ?
V1 Cs1A Cs1B O2 -153.70(3) 7_677 . . 1_655 ?
V1 Cs1A Cs1B O2 93.70(3) . . . 1_665 ?
V1 Cs1A Cs1B O2 -93.70(3) 1_655 . . 2_775 ?
V1 Cs1A Cs1B O2 153.70(3) 7_677 . . 3_665 ?
O1 Cs1A Cs1B Cs1B -90.0(2) 1_665 . . 7_777 ?
O1 Cs1A Cs1B Cs1B 90.0(2) 7_667 . . 7_777 ?
O1 Cs1A Cs1B Cs1B 150.00(1) 7_677 . . 7_777 ?
O1 Cs1A Cs1B Cs1B -30.00(1) 1_655 . . 7_777 ?
O1 Cs1A Cs1B Cs1B 30.0(2) . . . 7_777 ?
O1 Cs1A Cs1B Cs1B 30.00(1) 7_777 . . 7_777 ?
O1 Cs1A Cs1B O1 -60.000(0) 1_655 . . 7_777 ?
O1 Cs1A Cs1B O1 180.000(0) 1_665 . . 7_667 ?
O1 Cs1A Cs1B O1 60.000(1) 1_655 . . 7_667 ?
O1 Cs1A Cs1B O1 180.000(1) . . . 7_777 ?
O1 Cs1A Cs1B O1 120.000(1) 7_667 . . 7_677 ?
O1 Cs1A Cs1B O1 180.000(1) 1_655 . . 7_677 ?
O1 Cs1A Cs1B O1 -60.000(1) . . . 7_667 ?
O1 Cs1A Cs1B O1 60.000(1) . . . 7_677 ?
O1 Cs1A Cs1B O1 119.999(1) 7_777 . . 7_667 ?
O1 Cs1A Cs1B O1 60.001(0) 1_665 . . 7_777 ?
O1 Cs1A Cs1B O1 -120.000(0) 7_677 . . 7_667 ?
O1 Cs1A Cs1B O1 -120.000(1) 7_777 . . 7_677 ?
O1 Cs1A Cs1B O1 120.000(0) 7_677 . . 7_777 ?
O1 Cs1A Cs1B O1 -119.999(0) 7_667 . . 7_777 ?
O1 Cs1A Cs1B O1 -60.000(1) 1_665 . . 7_677 ?
O1 Cs1A Cs1B O2 93.70(3) 1_655 . . 2_665 ?
O1 Cs1A Cs1B O2 -93.70(3) 1_665 . . 3_565 ?
O1 Cs1A Cs1B O2 86.30(3) 7_777 . . 1_655 ?
O1 Cs1A Cs1B O2 -153.70(3) 7_677 . . 1_655 ?
O1 Cs1A Cs1B O2 -146.30(3) 1_655 . . 1_665 ?
O1 Cs1A Cs1B O2 -26.30(3) 1_655 . . 3_665 ?
O1 Cs1A Cs1B O2 -33.70(3) 7_777 . . 2_775 ?
O1 Cs1A Cs1B O2 -153.70(3) 7_777 . . 3_565 ?
O1 Cs1A Cs1B O2 153.70(3) 7_677 . . 3_665 ?
O1 Cs1A Cs1B O2 -33.70(3) 7_677 . . 3_565 ?
O1 Cs1A Cs1B O2 86.30(3) 7_677 . . 2_775 ?
O1 Cs1A Cs1B O2 146.30(3) 1_655 . . 3_565 ?
O1 Cs1A Cs1B O2 -153.70(3) 7_667 . . 2_775 ?
O1 Cs1A Cs1B O2 153.70(3) 7_667 . . 1_665 ?
O1 Cs1A Cs1B O2 93.70(3) . . . 1_665 ?
O1 Cs1A Cs1B O2 33.70(3) 7_667 . . 2_665 ?
O1 Cs1A Cs1B O2 33.70(3) 7_777 . . 3_665 ?
O1 Cs1A Cs1B O2 -146.30(3) 1_665 . . 2_665 ?
O1 Cs1A Cs1B O2 33.70(3) 7_677 . . 1_665 ?
O1 Cs1A Cs1B O2 -26.30(3) 1_665 . . 1_665 ?
O1 Cs1A Cs1B O2 26.30(3) . . . 3_565 ?
O1 Cs1A Cs1B O2 -86.30(3) 7_777 . . 1_665 ?
O1 Cs1A Cs1B O2 -93.70(3) 1_655 . . 2_775 ?
O1 Cs1A Cs1B O2 26.30(3) 1_655 . . 1_655 ?
O1 Cs1A Cs1B O2 146.30(3) . . . 2_775 ?
O1 Cs1A Cs1B O2 -93.70(3) . . . 1_655 ?
O1 Cs1A Cs1B O2 26.30(3) 1_665 . . 2_775 ?
O1 Cs1A Cs1B O2 153.70(3) 7_777 . . 2_665 ?
O1 Cs1A Cs1B O2 -86.30(3) 7_667 . . 3_665 ?
O1 Cs1A Cs1B O2 -33.70(3) 7_667 . . 1_655 ?
O1 Cs1A Cs1B O2 86.30(3) 7_667 . . 3_565 ?
O1 Cs1A Cs1B O2 146.30(3) 1_665 . . 1_655 ?
O1 Cs1A Cs1B O2 -86.30(3) 7_677 . . 2_665 ?
O1 Cs1A Cs1B O2 93.70(3) 1_665 . . 3_665 ?
O1 Cs1A Cs1B O2 -26.30(3) . . . 2_665 ?
O1 Cs1A Cs1B O2 -146.30(3) . . . 3_665 ?
O1 V1 O2 Cs1B -62.42(10) . . . 1_445 ?
O1 V1 O2 Cs1B 62.42(10) . . . 1_455 ?
O1 V1 O2 Cu1 -0.001(0) . . . 7_566 ?
O1 V1 O2 Cu2 180.0 . . . . ?
O2 Cu2 O3 Cu1 0.0 7_566 . . . ?
O2 Cu2 O3 Cu1 180.0 . . . . ?
O2 Cu2 O3 Cu2 -71.30(10) . . . 3_565 ?
O2 Cu2 O3 Cu2 71.30(10) . . . 2_665 ?
O2 Cu2 O3 Cu2 108.70(10) 7_566 . . 3_565 ?
O2 Cu2 O3 Cu2 -108.70(10) 7_566 . . 2_665 ?
O2 V1 O1 Cs1A 180.001(0) 3_565 . . 1_445 ?
O2 V1 O1 Cs1A 60.000(0) . . . 1_445 ?
O2 V1 O1 Cs1A -59.999(0) 3_565 . . . ?
O2 V1 O1 Cs1A 60.001(0) 3_565 . . 1_455 ?
O2 V1 O1 Cs1A 180.000(0) . . . . ?
O2 V1 O1 Cs1A -60.0 . . . 1_455 ?
O2 V1 O1 Cs1A -60.000(0) 2_665 . . 1_445 ?
O2 V1 O1 Cs1A 60.000(0) 2_665 . . . ?
O2 V1 O1 Cs1A 180.000(0) 2_665 . . 1_455 ?
O2 V1 O1 Cs1B -59.999(0) 3_565 . . . ?
O2 V1 O1 Cs1B -60.000(1) . . . 1_455 ?
O2 V1 O1 Cs1B 60.000(0) . . . 7_667 ?
O2 V1 O1 Cs1B -60.000(1) . . . 7_677 ?
O2 V1 O1 Cs1B 180.000(1) 2_665 . . 1_455 ?
O2 V1 O1 Cs1B 60.000(0) 2_665 . . . ?
O2 V1 O1 Cs1B 60.001(1) 3_565 . . 7_677 ?
O2 V1 O1 Cs1B 60.000(0) . . . 1_445 ?
O2 V1 O1 Cs1B -59.999(0) 3_565 . . 7_777 ?
O2 V1 O1 Cs1B -60.000(0) 2_665 . . 1_445 ?
O2 V1 O1 Cs1B 60.000(1) 2_665 . . 7_777 ?
O2 V1 O1 Cs1B 60.001(1) 3_565 . . 1_455 ?
O2 V1 O1 Cs1B 180.000(1) 2_665 . . 7_677 ?
O2 V1 O1 Cs1B 180.000(0) . . . 7_777 ?
O2 V1 O1 Cs1B -60.000(1) 2_665 . . 7_667 ?
O2 V1 O1 Cs1B 180.001(0) 3_565 . . 7_667 ?
O2 V1 O1 Cs1B 180.001(0) 3_565 . . 1_445 ?
O2 V1 O1 Cs1B 180.000(0) . . . . ?
O2 V1 O2 Cs1B 57.51(12) 2_665 . . 1_445 ?
O2 V1 O2 Cs1B -177.64(11) 2_665 . . 1_455 ?
O2 V1 O2 Cs1B 177.64(11) 3_565 . . 1_445 ?
O2 V1 O2 Cs1B -57.52(12) 3_565 . . 1_455 ?
O2 V1 O2 Cu1 119.94(6) 2_665 . . 7_566 ?
O2 V1 O2 Cu1 -119.94(6) 3_565 . . 7_566 ?
O2 V1 O2 Cu2 60.06(6) 3_565 . . . ?
O2 V1 O2 Cu2 -60.06(6) 2_665 . . . ?
loop_
_exptl_oxdiff_crystal_face_indexfrac_h
_exptl_oxdiff_crystal_face_indexfrac_k
_exptl_oxdiff_crystal_face_indexfrac_l
_exptl_oxdiff_crystal_face_x
_exptl_oxdiff_crystal_face_y
_exptl_oxdiff_crystal_face_z
0.9999 -0.9957 0.0035 0.0088 -0.0101 0.1273
8.7213 -6.2910 0.2386 -0.0911 0.1375 0.9863
-0.1631 7.8757 -0.1134 -0.4873 0.7653 -0.4205
2.2040 -8.6604 0.1595 0.4227 -0.6651 0.6156
-6.8821 -1.5828 -0.0964 0.4846 -0.7566 -0.4390
-7.8233 7.7680 -0.2438 -0.0522 0.0869 -0.9948
0.2150 -0.1982 -11.8179 0.8428 0.5382 0.0091
-0.2150 0.1982 11.8179 -0.8428 -0.5382 -0.0091
7.1016 -6.2837 5.9744 -0.4116 -0.2657 0.8718
0.5176 6.4665 5.9380 -0.8654 0.4107 -0.2870
2.5831 -6.4706 8.1629 -0.3084 -0.7813 0.5427
-1.5952 -3.5774 9.5583 -0.3646 -0.9279 0.0786
